Download presentation

Presentation is loading. Please wait.

Published byDiana Graves Modified over 2 years ago

1
1 ASTM : American Society of Testing and Materials

2
2 Assuming a small plastic zone compared to the specimen dimensions, a critical value of the mode-I SIF may be an appropriate fracture parameter. K IC : plane strain fracture toughness plane strain K C : critical SIF, depends on thickness plane stress K I > K C : crack propagation Specimen Thickness KCKC K IC : Lower limiting value of fracture toughness K C Material constant for a specific temperature and loading speed Introduction:

3
3 Standard Test Methods for Plane-Strain Fracture Toughness and Strain Energy Release Rate of Plastic Materials K I based test method ensures that the specimen fractures under linear elastic conditions confined plastic zone at the crack tip Many similarities to E 399, with additional specifications important for plastics. ASTM E 399 first standardized test method for K IC : - was originally published in 1970 - is intended for metallic materials - has undergone a number of revisions over the years - gives specimen size requirements to ensure measurements in the plateau region ASTM D 5045 -99 is used here for plastic materials:

4
4 Two specimen configurations for D 5045 -99 : Three Point Bend specimen (SENB): Compact tension configuration (CT): 1- Test specimens

5
5 For valid K IC measurements, the specimens are designed to ensure : B must be sufficient to ensure plane strain. yield stress of the material for the temperature and loading rate of the test W-a must be sufficient to avoid excessive plasticity in the ligament. - a small plastic zone size / specimen thickness B. - that plane strain conditions dominate around the crack tip. Plastic zone length c from Irwin Model (plane strain): Plane stress condition if c = B From ASTM 399 Plane strain condition if c < B/25 Thus,

6
6 2- Precrack: K C decreases with decreasing until a limiting value C 6.3 m The theory considers an ideal plane crack with zero notch radius Notch in reality Below C, K C approximately constant: The notch can simulate the theoretical crack Remark:

7
7 Chevron starter notch (see p4-26): The chevron forces crack initiation at its center. A sharp crack of length a f is propagated by fatigue such that: where Natural crack a0a0 W a The measured crack length a is the average of the crack lengths measured at: - the center of the crack front: a 1 - the end of the crack front on each surface: a 2 and a 3 During fatigue the maximum SIF must not exceed 60 % of K IC B a1a1 a2a2 a3a3 B W Measurements of B and W to 0.1% accuracy Alternatively, a2a2 a3a3 B W a1a1

8
8 Laboratory specifications for the specimen W = 48 mm a 0 = 0.45 W A A A-A B Chevron 90°

9
9 3- Experimental procedure Expression for the calculation of the SIF (CT- configuration): f shape function for the CT specimen (see A2.5 p8) Accurate within ± 0.65% over the range K Q conditional or trial K IC value. Fatigue crack propagation: P(t) 30 120 Time P(t) (N) half a day to complete 3 Hz Crack front

10
10 Servohydraulic testing system (Instron) used with constant displacement rate imposed. Several specimens tested (at least three) : reproducibility Both displacement and load recorded simultaneity during the test. Loading rate and test temperature should be noted. Test procedure: (see section 8.3)

11
11 4- Interpretation of test record and calculation of K IC P max : maximum load sustained by the specimen AB : initial compliance C = u / P AB’ : compliance 5% greater than AB Evaluation of P Q : P max within lines (AB) and (AB’): P Q = P max P max outside lines (AB) and (AB’): P Q = intersection of (AB’) and the load curve Calculus of K Q P max / P Q < 1.1 Calculus of K Q P max / P Q > 1.1 Test invalid

12
12 Calculation of the trial value K Q with the relation : If moreover, then is equal to When the test result fails to meet these requirements, use a 1.5 times larger specimen. (see 9.1.5) See Testing summary table 3, p6. http://lmafsrv1.epfl.ch/Fracture_course2006/KIC%20testing/

13
13 Typical K IC values:

Similar presentations

Presentation is loading. Please wait....

OK

ASPECTS OF MATERIALS FAILURE

ASPECTS OF MATERIALS FAILURE

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on carbon and its compounds worksheet Download ppt on indus valley civilization pictures Micro display ppt online Free ppt on moving coil galvanometer instrument Ppt on airbag working principle of motor Conceptual architecture view ppt on android Ppt on thermal power plant working Ppt on rational and irrational numbers for class 9 Ppt on product data management Ppt on success after failure